Discussion Chain ID: 109887
================================================================================

User asked: How can I prevent my spin-coated silica thin film from cracking when I heat it up?

I am spin-coating a porous silica solution on a glass microscope coverslip, and then heating the resulting thin film to $\pu{350 °C}$, in an attempt to create a thin film of porous silica sol gel. I am trying to replicate _only the porous sol gel portion_ of the work of Yantasee et al.: [Nanoengineered electrochemical sensor based on mesoporous silica thin-film functionalized with thiol-terminated monolayer](https://pubs.rsc.org/en/content/articlehtml/2003/an/b303973k) The problem I am encountering is that my heated sol gel is cracking and partially delaminating. This is unacceptable. Can anyone offer advice on how to prevent this cracking when heating to $\pu{350 °C}$? **Relevant Information** 1. The recipe for the silica precursor solution is: 2.578 g quantity of Pluronic F-127 surfactant was dissolved in 3.430 g of deionized water and 8.846 g of ethyl alcohol. Then 0.108 g of concentrated $\ce{HNO3}$ was added into the mixture. Finally, a 5.0 g quantity of TEOS was added to the solution. 2. The solution was sonicated for 8 hours and then spin-coated at 3000 rpm onto the surface of a 12 mm glass microscope cover slip. 3. Film thickness: ~10 μm. **Possible Causes** * Perhaps I am using the wrong type of glass for the substrate, and the respective thermal expansions are causing cracking at the interface. If so, what relatively cheap glass could I use? * Maybe I need to rigorously prepare the glass substrates by cleaning them with a solution of acid (or base) and solvent. Could an ill-prepared substrate contain contaminants acting as nucleation sites for crack formation when heated? If so, what best method is used by these groups to prepare their slides? I can't seemed to find a paper on sol gel thin films where they describe their substrate preparation.

Discussion:
Comment: I suggest trying the thermal treatment without placing the glass slide in direct contact with the hottest walls of the furnace and focus on a T ramp. These kind of problems are normal and rarely mentioned in experimental parts as for their description and work around are generally looking childish ;) as for most of the users are from disparate fields of chem and phys. You can also contact an author. Normally s/he will answer telling you how no to crack the film. I colleague of mine struggled with TiOx, I suspect he was just making so many films that he did find some of them usable.

Answer 1 (1 votes):
The reference you sited has used gold surface to make the thin film. If the method you wanted is the one in that reference, folloeing is how they descibed it in experimental section: > The modification of a gold electrode array on microchip with a SH-FMS thin film consisted of two steps. First a mesoporous silica film was deposited onto the electrode surface by the spin-coating technique. Then the thiol functional groups were immobilized inside the mesopores of the film by self-assembly chemistry. To prepare the silica film solution, a 2.578 g quantity of Pluronic F-127 surfactant was dissolved in 3.430 g of de-ionized water and 8.846 g of ethyl alcohol. Then 0.108 g of concentrated HNO3 was added into the mixture. Finally, a 5.0 g quantity of TEOS was added to the solution. The molar ratio of TEOS : water : ethanol : HNO3 : Pluronic F-127 was 1 : 8 : 8 : 0.05 : 0.008. The solution was shaken for 24 h, then spin-coated at the speed of 3000 rpm onto the bare surface of a gold microelectrode array on microchip (part No. M1450110, Microsensor System, Inc.) for 30 s. Fig. 1a shows the schematic of the microelectrode array. The specific electrode array had 50 finger pairs (15 microns finger width and finger spacing) with gold as the electrode material and quartz as the substrate. The electrical connection for the array was covered with plastic tape before spin coating with the film solution. After the spin coating, the tape was removed and the film-coated electrode was calcined on a hot plate at 350 °C for 8 min in air. Hope this is helpful.

Answer 2 (1 votes):
I have encountered similar issue while spin coating thin film of NiO. In my case, following steps resolved the problem: 1. Preheating the substrate for 1 min at 100°C 2. After the solution is coated on the substrate, drying it in pre heated oven for 10 min at 120 °C (My solvent was 2 methoxy ethanol) 3. Then calcining in furnace at required temp. The ramp rate should be taken into account. Thanks and Regards

Discussion on this answer:
Comment: Doesn't the sample cool dwon from 100°C --> room temp during the spin coat, since you have to remove it from the hotplate? Is the substrate still warm at the start/after the spin-coat? I suspect the reason this worked is the common glass-manufacturing trick to zig-zag ramp your temperature up to full temp.

Answer 3 (0 votes):
I agree that your substrate's CTE mismatch is the cause, in addition to the thickness you're coating (thicker film == more total force of delamination). You could reduce the thickness of the coated film to reduce thin-film force. Or increase adhesion - for axample, try and Oxygen or Argon plasma activation on the substrate to make the surface hydrophilic (very tolerant - basically any power and >10sec plasma etch would work). Lastly, you could try a gradual/zig-zag temperature ramp up protocol, such as: * coat substrate * heat up to 100°C over ~5min then cool down over ~5min * heat up to ~200°C over ~5-10min then cool down over ~5-10min * heat up to ~350°C over ~10min then cool down over ~10min These are just guesses, but modifications of the general thermal profile strategy might help.


================================================================================

